Author's Accepted Manuscript
Separation of butanol from ABE mixtures by sweep gas pervaporation using a supported gelled ionic liquid membrane: Analysis of transport phenomena and selectivity A. Plaza, G. Merlet, A. Hasanoglu, M. Isaacs, J. Sanchez, J. Romero
PII: DOI: Reference:
S0376-7388(13)00314-1 http://dx.doi.org/10.1016/j.memsci.2013.04.034 MEMSCI12091
To appear in:
Journal of Membrane Science
Received date: 26 December 2012 Revised date: 2 April 2013 Accepted date: 11 April 2013 Cite this article as: A. Plaza, G. Merlet, A. Hasanoglu, M. Isaacs, J. Sanchez, J. Romero, Separation of butanol from ABE mixtures by sweep gas pervaporation using a supported gelled ionic liquid membrane: Analysis of transport phenomena and selectivity, Journal of Membrane Science, http://dx.doi.org/ 10.1016/j.memsci.2013.04.034 This is a PDF file of an unedited manuscript that has been accepted for publication. As a service to our customers we are providing this early version of the manuscript. The manuscript will undergo copyediting, typesetting, and review of the resulting galley proof before it is published in its final citable form. Please note that during the production process errors may be discovered which could affect the content, and all legal disclaimers that apply to the journal pertain.
Separation of butanol from ABE mixtures by sweep gas pervaporation using a supported gelled ionic liquid membrane: analysis of transport phenomena and selectivity
Plaza, A.1, Merlet, G.1Hasanoglu, A.1,2, Isaacs, M.3, Sanchez, J.4, Romero, J.1*
1) Laboratory of Membrane Separation Processes (LabProSeM), Department of Chemical Engineering, University of Santiago de Chile (USACH). 2) Yldz Technical University, Department of Chemical Engineering, Davutpaa, 34210 Istanbul, Turkey. 3) Department of Inorganic Chemistry, Faculty of Chemistry, Catholic University of Chile (PUC). 4) Institut Europeen des Membranes (IEM UMR 5635, UM2/ENSCM/CNRS)
ABSTRACT The separation of acetone-butanol-ethanol mixtures (ABE) from aqueous solutions, which are produced in ABE fermentation processes, is carried out by sweep gas pervaporation using gelled supported ionic liquid membranes and by membrane evaporation. The membranes were synthetized by the gelation of an ionic liquid ([bmim][PF6]) into the porosity of polytetrafluoroethylene (PTFE) hollow fibers. The performance of the membranes used in sweep gas pervaporation is compared with the membrane evaporation process using the same hollow fiber support without IL in order to verify the selectivity contributed by the gelled ionic liquid gap formed in the membrane pores. Improved butanol/ethanol selectivity was verified for gelled IL membranes in pervaporation experiments compared to the evaporation process. A
resistance-in-series model was developed to simulate the pervaporation process. The model predictions were in good agreement with the experimental results. IL membranes are found to have potential for separation of butanol from the ABE mixtures by pervaporation.
Keywords: Pervaporation; butanol; supported liquid membranes; gelled ionic liquid; mass transfer.
*: Corresponding author: Dr. Julio Romero Department of Chemical Engineering, University of Santiago de Chile (USACH) E-mail: [email protected]
Tel: +56 2 718 18 21 1.- Introduction The use of alternative fuels has gained attention recently because of the increasing energy demands, future limitations in the oil resources and correspondingly increase in fuel prices, and the negative environmental effects of the gases produced in the petroleum industries. There is great potential for the use of biofuels in industrial applications, such as heat and power generation and transportation sector. Bio-butanol has been considered as a promising alternative fuel that can be produced from renewable resources. It has several advantages over other low-carbon bio-alcohols such as: low volatility, high heating value, easy partition in the base fuel, and no ignition problems . ABE fermentation is a butanol production process that employs a strain of bacteria from the Clostridium family to fermentate a starch substrate, sugar beets, glucoses, cellulosic-based materials and other biomass feedstocks. This process to
produce butanol was very used during the first part of the 20th century [2, 3] and it has gained attention again lately due to the depletion of fossil fuels. Primary products of ABE fermentation are acetone, butanol, and ethanol often in a 3:6:1 ratio. Pervaporation has a great potential to recover the butanol from the fermentation broth, since this process does not have harmful effects on the fermentation culture, besides it is a one-step single process that can be coupled to the fermentation unit easily. The recovery of butanol by pervaporation has been investigated in several works. Various membranes have been used for butanol separation from fermentation broths, membranes were made from different materials such as polydimethylsiloxane (PDMS), zeolite or silicalite-filled siloxane [4-12], polypropylene [13, 14], poly(ether-blockamide) [15, 16], poly(vinylidene fluoride)  and ceramic composites of PDMS [18, 19]. Moreover, pervaporation could enhance continuous ABE fermentation, since this process would allow the continuous extraction of the produced solvents. In batch configuration, the final concentration obtained for combined solvents in the fermentation broths cannot be higher than 25000 ppm  because the viability of Clostridium bacteria is affected by high concentrations of the products. Butanol tolerance of bacteria used in fermentation is an important aspect that affects the production costs of biobutanol. Low concentration of butanol in the fermentation broth causes high product recovery costs . Butanol toxicity is mainly caused by its hydrophobic nature, which increases the fluidity of the cell membrane. Thus, the function of the cell membrane as a controlling barrier between cell interior and exterior can be affected.
From the results of tests developed by Knoshaug and Zhang [21, 22] on 24 microbial species, only 4 were able to grow at the butanol concentration of 2 wt% and the growth rate was <20% of the obtained one with no butanol present. On the other hand, Ionic liquids (ILs) are considered a new class of green solvents, which shows several advantages over conventional solvents such as a negligible vapor pressure and the capacity to solvate a variety of organic and inorganic species. Many of the ILs are both air and moisture stable. However, this depends on the hydrophilic/hydrophobic character of the IL. The degree of the hydroscopic character of the IL and consequently the interaction between water and IL is strongly depended on anions of the IL. The use of ILs in membrane techniques has been investigated with promising results . Although ILs have a good potential for butanol separation and they have been used for various applications of butanol separation in the literature, such as liquid-liquid extraction or recovery from transesterification reaction [24-29], however the application of IL membranes for separation of butanol from ABE solvents by pervaporation has not been fully investigated. Izák and coworkers  studied selective removal of acetone and butanol from water with supported ionic liquid– polydimethylsiloxane membrane by pervaporation. They compared an ultrafiltration membrane impregnated by the ionic liquid and PDMS with a classical dense PDMS membrane. They used two different ionic liquids; 1-ethenyl-3-ethyl-imidazolium hexafluorophosphate and tetrapropylammonium tetracyanoborat. They reported that the use of ILs enhanced the selectivity. Cascon and coworkers  investigated various hydrophobic ionic liquids with high potential as butanol extractants, determining its butanol partition coefficient values, Kp, and their toxicity to solventogenic Clostridia species using ABE model solutions. Ammonium and phosphonium cation-based ionic
liquids were tested and it was indicated that all extractants showed the same Kp trend for typical fermentation products: butanol > acetone > ethanol. The coupling of ionic liquids and membrane techniques usually requires an impregnation of the IL by stabilizing it into a porous support matrix to prevent leaks under applied pressures that might be caused by mechanical strength problems. In pervaporation process the use of ionic liquid suffers from being displaced at relatively low differential pressures. Pervaporation membranes should show an improved mechanical stability, decreasing the possibilities of IL losses from the membrane pores, especially under the eventual high trans-membrane pressure gradient applied in this type of process. One solution to this drawback is the stabilization of ILs by gelation. Indeed, ILs can be stabilized by gelation by using several polymeric materials or gelation agents giving materials with good mechanical strength and conductivity and even enhancing their physico-chemical properties [32, 33]. Voss and coworkers presented a new type of IL material for CO2 separation based on physical gelation of [C6mim] [Tf2N] with 12hydroxystearic acid as a low-molecular-weight organic gelator . They reported that good mechanical strength is achieved with the resulting gelled IL membranes. In this work, we used the [bmim][PF6] to prepare IL gels using 12hydroxystearic acid gelator. The gelation methodology was adapted to prepare supported gelled IL membranes using macro porous PTFE hollow fibers as support. The resulting supported gelled IL membranes were tested in terms of butanol recovery from ABE solvents by using a non-classical pervaporation configuration: sweep gas pervaporation, in this process the upstream and downstream compartments are maintained at the same pressure but in the last one a continuous flow of nitrogen is swept in order to maintain a high concentration gradient while ensuring the stability of the IL gel. This process was compared to a membrane evaporation process [34, 35],
which is based on the transfer of vapors through the hydrophobic membrane porosity (without IL) by using also a continuous flow of nitrogen downstream in order to maintain a high concentration gradient. In the literature, it was not encountered a specific study to investigate butanol separation using ME. In this study, ME was implemented with the same membrane support used in pervaporation experiments with supported IL membranes in order to obtain a standard response with a non-selective membrane. The stability of the IL membranes was investigated evaluating the separation performance with time. Effect of the operating parameters on the pervaporation process was also investigated. A resistance-in-series model was developed to describe mass transfer through the membranes. 2.- Experimental 2.1. Material The
(synthesis grade), 12-hydroxystearic acid (purity 99% w/w) and acetone, butan-1-ol and ethanol (analytical grade) were supplied by Merck, Sigma-Aldrich and Equilab, respectively.
2.2. Membrane preparation 2.2.1. Preparation of IL gels Preliminary experiments were carried out to assess the formation of gels with the [bmim][PF6]. For this purpose we used the method described by Tan and co-workers , but in our case the chosen low molecular weight gelator was 12-hydroxystearic acid. This gelator had been already used for the synthesis of dense IL membranes for gas separation . In order to avoid excessive extend of condensation or cross-linking
reactions, which could result in a significant decrease in the transport properties of the IL gel, the gel preparation was achieved with a relatively low concentration of gelator (0.4% w/w). However, this small amount of gelator ensured the mechanical stability of the gel. In order to prepare the IL gel, the gelator is dissolved in the ionic liquid and kept in a ultrasonic bath 4 h at 800C. Some preliminary experiments were carried out with and without gelator in the IL impregnated module in order to see the effect of the gelator on the mechanical stability of the membrane. When gelator was not used, the ionic liquid passed to the feed, which could be observed as a formation of two phases in the vessel that contained the feed solution. On the other hand using gelator this problem was overcame and no permeation of ionic liquid was observed.
2.2.2. Preparation of single fiber PV membrane module For the preparation of the IL membrane a polytetrafluoroethylene (PTFE) hollow fiber supplied by GoreTex™ was placed in a stainless steel housing and its ends were glued with an epoxy resin. Table 1 summarizes the structural parameters of the PTFE porous fiber used in this work. Figure 1 shows the outline of a cross-section of a gelled ionic liquid membrane supported in a porous hollow fiber. For the introduction of the IL gel into the pores of the PTFE fiber, the membrane housing was kept at 80°C with an electric tape and a flow of IL-gelator mixture was circulated into the lumen-side using a peristaltic pump while vacuum was applied on the shellside by means of a vacuum pump until a constant permeation flow was observed. Then a flow of nitrogen was simultaneously introduced in the lumen and shellside in
order to clean all the excess gelator-IL mixture. The temperature of the module was then decreased from 80ºC to 20ºC at a rate of 10ºC/min. The volume of the IL mixture circulated through the membrane was 10 ml. In order to obtain membrane stability in the module in time, the same experiment was repeated using the same module several times until the selectivities begun to change. Until first 5-6 experiments the selectivities were consistent, after then the separation performance begun to decrease and gave similar results to the membrane evaporation in which no IL was included in the pores. This showed that membrane stability changes after a period of usage. Therefore, the modules were used maximum 4 times for experiments to ensure the membrane provides the same separation performance for all experiments.
2.3. Pervaporation and membrane evaporation experiments: experimental setup The first process studied was the sweep gas pervaporation using a membrane based on supported ionic liquid gel. The objective was to characterize the mass transfer in the separation of acetone, butanol and ethanol from aqueous solutions using a pervaporation process. The performance of the sweep gas pervaporation process was then compared with a membrane evaporation operation using the same membrane support, but without ionic liquid gel filling its pores. In this way, the fluid dynamic aspects of the mass transfer can be isolated in order to identify the selectivity of the IL membrane itself. The objective of the comparison of PV and ME is to show the effect of the IL on the selectivity since ME is practically the same operation of PV without IL in the pores. To exhibit the effect of the IL on the selectivity, all the fluid dynamic aspects were kept the same in two operations showing that the improvement of the selectivity could be only caused by the presence of the IL in the pores. Thus, the experimental
device built in this work allows comparing both processes using different membranes: with or without ionic liquid gels inside the pores, but maintaining the same circulation configuration. The outline of the experimental setup is shown in Figure 2. Sweeping gas pervaporation experiments were done to separate the solutes acetone/butan-1-ol/ethanol from aqueous solutions containing 500 ppm of each compound. Pervaporation runs were done using the experimental setup described in Figure 2, circulating the aqueous solutions into the lumen-side of the hollow fiber membrane with flow rates ranged from 1.2x10-3 to 3.0x10-3 L.min-1. On the shellside, nitrogen was flowed in countercurrent flow with rates varying between 0.6 and 1.3 L min-1. A vessel with cold water was used to receive the components of the sweep gas for security cautions by bubbling the gas into the water. The pervaporation system was operated under transient conditions. Thus, the concentration decrease of acetone, butanol and ethanol in the feed solution with time was monitored by chromatographic analysis by using a Perkin Elmer Clarus 500 gas chromatograph, a Carbowax 20M column and a FID detector. Pervaporation experiments were done for 75 min. In this way, extraction percentage of the compounds during the experiment was calculated by monitoring the concentration change in the feed every 15 minutes. The average transmembrane fluxes of the components were calculated using a mass balance around the membrane monitoring the volume decrease of the feed at the end of the experiment. The permeation flux and selectivity depended on time could not be measured at certain time intervals of the experiment since the amounts were to small to analyze, but instead, the average fluxes of the components were obtained at the end of the experiment using a mass balance monitoring the volume decrease.
The extraction percentage of a compound from feed solution was calculated from the equation below: (1)
where CS,,f(aq)(t=0) is the initial concentration of the compound and CS,,f(aq)(t) is the concentration in feed at any time. Moreover the trans-membrane flux (kg m-2 h-1) of each compound was calculated with the following equation: (2)
where NSEXP is the trans-membrane flux of solute (kg m-2 h-1), Vf is the total volume of the liquid feed solution in the system, SID is the interfacial surface area (m2) available for the mass transfer. The derived function in equation 2 is obtained from the experimental results and the numerical derivation of the empirical correlation curve. The operating conditions are summarized in Table 2. As explained above, the effect of the IL gel in the fibers on separation performance was investigated comparing the results with and without IL in the fiber by using identical configurations and conditions for sweeping gas pervaporation and with membrane evaporation processes.
3.- Mass transfer model 3.1. Mass transfer steps for sweep gas pervaporation The mass transfer model proposed for the sweep gas pervaporation is based on a resistance-in-series model, which represents each transport step at the proximities of the supported membrane. Thus, three transfer steps can be identified: 1) Convection through the boundary layer of the aqueous feed stream containing acetone, butanol and
ethanol; 2) molecular diffusion of solutes through the ionic liquid gel layer formed into the pores of the membrane support; and 3) convection through the boundary layer of the stripping gas phase. Between steps 1-2 and 2-3 a thermodynamic equilibrium conditions were considered. These equilibrium conditions involve the absorption and desorption of the three solutes to and from the ionic liquid gel layer, respectively. Mass transfer at the proximities of the membrane and the concentration profile are represented in Figure 3a. From these assumptions, the mass transfer flow (kg h-1) of each solute can be estimated by the following equations:
Equations 3, 5 and 7 represent the mass transfer flux through the aqueous feed solution boundary layer, the ionic liquid gel gap retained in the pores and gas stream boundary layer, respectively. In equation 5, the surface of the IL was calculated based on the logarithmic mean diameter. Equations 4 and 6 define the partition coefficient for IL gel/aqueous phase and IL gel/gas stream, respectively. kaq and kg are the mass transfer coefficients of aqueous and gaseous boundary layer, respectively. These
coefficients can be estimated by equations based on Reynolds, Schmidt, and Sherwood dimensionless numbers . KIL/aq and KIL/g are the partition coefficient between the aqueous solution-IL gel and the gel IL-N2, respectively. The mass transfer rate inside the pores occurs through a diffusive mechanism, which can be quantified through the effective mass transfer coefficient into the pore filled with gel ionic liquid, kp-IL. This mass transfer coefficient in equation 5 can be estimated by means of the equation 8 [38, 39]: (8) where DS,IL is the diffusion coefficient of the solute in the gelled IL layer that fills the pores of the supporting membrane, is the porosity, is the tortuosity and L is the thickness of the hollow fiber support. It was assumed that solute transfer through the PTFE was negligible. This could be considered acceptable, since the diffusion coefficient of this compounds in solids such as PTFE are 4 orders of magnitude lower than its values in liquids. Under steady-state conditions, the mass transfer flow (mol s-1) values estimated form equation 1, 3 and 5 must be identical. In this work, the mass transfer model is solved under a pseudo steady state condition, which is supposed for each time step. The mass balances of the solutes are done after every time step in order to estimate the concentration change in the aqueous feed solution as a function of the time. The numerical solution is explained in detail in section 3.4. The contribution of each local transport step on the overall transfer rate can be estimated from the equation that allows the calculation of the overall mass transfer coefficient, KTPervap, written as a resistances-in-series model :
Equation 9 considers the contribution given by the aqueous feed solution boundary layer and the gelled IL layer in the pores. In this case, the contribution of the gas stream boundary layer is neglected because this phase shows transport parameters higher than the considered ones . Thus, the mass transfer resistance fraction of the aqueous feed boundary layer and the gelled IL membrane can be estimated by means of the equations 10 and 11, respectively. (10)
3.2.- Physical and transport properties The Leveque’s equation has been used for the calculation of the Sherwood number and then the mass transfer coefficient Kaq of a fluid flowing inside a cylindrical pipe [37,38,41]: (12)
This equation can be used to predict the mass transfer coefficient on a fluid circulating inside a tube in laminar regime, with good precision at Gz > 4.0. However, the coefficient is overestimated when Gz < 4.0. In the studied system, the Gz number values in the lumenside were ranged between 31.70 and 117.74.
To calculate the mass transfer coefficient
for a circulating flow inside the
housing (coaxial tubes), Gabelman et al. , proposed the following equation: (13)
Some physical properties of the components are given in Table 3.
3.3.- Mass transfer model for membrane evaporation In the case of membrane evaporation, the mass transfer principle of the process at the proximities of the membrane is explained in the Figure 3b above. In this case, membrane pores are empty and the transfer inside the pores is carried out through diffusion in the gas phase that fills the pores. By similitude with the case of IL membrane above, the mass transfer can be then described in 3 steps: 1) Convection through the boundary layer of the aqueous feed stream containing acetone, butanol and ethanol; 2) molecular diffusion of solutes through membrane pores filled with gas; and 3) convection through the boundary layer of the stripping gas phase. Between the steps 1-2 thermodynamic equilibrium conditions must be considered. In this case, the phase equilibrium can be assessed supposing Henry’s law, since the aqueous solution can be considered diluted for each solute. The first mass transfer step can be estimated by means of the same equation 1 proposed to describe the aqueous feed boundary layer in the model for pervaporation. After that, the phase equilibrium between feed solutions and stripping gas must be considered. Thus, a partition coefficient can describe this step. As far as in this process we are considering low solute concentrations and atmospheric pressure, it is possible, then, to utilize the ideal dilute solution model; therefore, the equilibrium expression can be simplified using Raoult’s law and Henry’s constant:
where Hg/aq is the Henry’s constant (dimensionless) of the solute of interest. CS,i1(g) and CS,i1(aq) are the concentrations of solute at the gas-liquid interface in the gas and aqueous phase, respectively. The second step concerns the mass transfer inside the pores. The hollow fibers used as supporting membranes are macroporous, for this reason mass transport could be described by molecular diffusion [37, 41]. Thus, trans-membrane flow inside pores can be described by: (15)
where CS,PORE(g) is the solute concentration in the boundary layer outside the pore. Finally, trans-membrane flow from the boundary layer outside the pore to the bulk aqueous phase can be described by the following equation: (16)
where CS,b(g) is the solute concentration on the bulk gas phase. Analogously to the resistance-in-series approach applied to pervaporation, the overall mass transfer for membrane evaporation, KTME, can be estimated by equation 17 : (17)
From equation 17, the mass transfer resistance fraction of the aqueous feed boundary layer, the membrane pores filled with gas and the gas stream boundary layer can be estimated by means of equations 18, 19 and 20, respectively.
For the solution of the resistances-in-series models for both pervaporation and membrane evaporation, the following assumptions have been considered: -
The aqueous solution is considered as a diluted solution; therefore it has a binary
Mass transfer through the membrane pores occurs through diffusion, which is generated by the concentration gradient, validating Fick’s law.
Physical properties of the solutions are considered constant.
No distortion of the velocity and concentration profile due to the mass transfer.
The thickness of the boundary layer is assumed constant along the membrane’s wall.
Laminar flow is considered in the shellside and lumenside.
The interfaces generated in pore’s mouths (aqueous/gas in the case of evaporation and aqueous/IL in the case of sweeping gas pervaporation) are considered as stable in time.
A negligible pressure drop along the module.
The system works in laminar regime and was adjusted according to cylindrical geometry.
In the sweep gas pervaporation process, the solute concentration on the ionic liquid-nitrogen boundary layer is considered equal to zero.
In membrane evaporation the concentration of the solute to be transferred into the bulk of the gaseous phase is considered to be very low, and then the bulk concentration is almost equal to zero.
3.4.- Numerical solution for transient state A simulation algorithm has been developed in Matlab®. It allows the evaluation of the permeate flux in function of the operation variables; this flux is determined for the individual coefficients in each resistance layer. In the first step, the operating conditions (flows rates of aqueous and gaseous solutions, composition, pressure and temperature) and the structural parameters (inside and outside diameters, membrane characteristics: length, porosity, tortuosity) are defined, while in the second step the program computes the properties of the phases and then calculates the dimensionless numbers and individual coefficients of mass transfer. Finally, in the last step the simulation program generates the estimation of transmembrane fluxes performing iteration of the concentrations at the interphases with the Regula Falsi method. This iteration was carried out to estimate interfacial concentrations for each time interval by modifying the concentrations at the pore entrances. Once interfacial concentration was known, the fluxes of each step could be calculated. When the estimated error is lower than the pre-established value the iterative algorithm is stopped and the transmembrane fluxes are identified. Figure 4 shows the flow sheet of this algorithm.
4.- Results and discussion 4.1.- Performance of the reference system: sweep gas membrane evaporation process
The first step in the characterization of the mass transfer through the pervaporation membrane is the quantification of fluid dynamic effects. For this purpose, the same experimental device was used to implement preliminary tests of sweep gas membrane evaporation of aqueous acetone-butanol-ethanol mixtures with the same PTFE hollow fiber, which was used as the membrane support in pervaporation tests. Thus, the non-selective support was used under the same fluid dynamic conditions of pervaporation tests in order to identify the real selectivity of the gelled supported ionic liquid membrane. As explained in the previous sections, experiments were carried out under transient conditions and the extraction percentage for both pervaporation and membrane evaporation was calculated using the equation (1), which gives the cumulative extraction in function of time. The experimental change of extraction percentages for each component in the mixture during the membrane evaporation process at different liquid and gas flow rates are shown in Figure 5. Figure 5 shows that acetone is extracted faster than ethanol and butanol, which both present similar extraction rates. The different extraction percentages are consistent with the comparative Henry’s constants of each compound, which is a function of volatility and solubility of a component in a mixture in equilibrium. Figure 6 shows the direct relationship between the mean transmembrane fluxes (kg h-1 m-2) obtained from experiments and Henry’s constant for each solute . Thus, the magnitude of transfer flows shows the same trends of the Henry’s constant, which can give information about volatility. Despite the fact that acetone shows the highest relative volatility, its mean transfer flux is not proportionally higher due to its mobility capacity into the membrane pores filled with gas and through the fluid phase boundary layers at the proximities of the membrane. In this way, ethanol is the smallest molecule and it shows diffusion coefficients in water and nitrogen higher than the ones show acetone and butanol. The
diffusion coefficient of ethanol in water is 1.58x10-9 m2s-1 while those of butanol and acetone are 1.23x10-9 m2s-1 and 1.42x10-9 m2s-1, respectively  under the experimental conditions chosen in this work. On the other hand, the diffusion coefficient of ethanol, butanol and acetone in nitrogen are 1.54x10-5, 1.23x10-5 and 1.37x10-5 m2s-1, respectively . However, extraction rates of ethanol and butanol are comparable, although the Henry’s constant for ethanol is comparatively lower. Similar evaporation rates of butanol and ethanol represent a technical problem in the obtaining of bio-butanol for the separation processes driven by vapor-liquid equilibrium such as distillation due to the presence of an azeotrope of these compounds, which presents a limitation in the separation. The mass transfer model based on a resistances-in-series approach was implemented to describe the extraction rate of each solute in the membrane evaporation process. Thus, the transfer of acetone, butanol and ethanol were individually described considering the transfer through the boundary layer of the liquid feed solution, the phase equilibrium at liquid-gas interface at the pore entrance and the diffusion of each solute across the membrane pores. Henry’s constants reported in Figure 6, were used in the mathematical model to describe the liquid-gas equilibrium at the pore entrance. In this theoretical description, the transfer resistance of gas stream was neglected because the high nitrogen flow resulted in very low bulk solutes concentration in this stream and then considered equal to zero. The results of these simulations are shown in Figure 7 where the concentration change rates are reported for each solute. A good agreement between experimental data and model predictions was observed from these results for all the operating conditions considered in this work, allowing to validate two main ideas: 1) the transfer through the proximities to the membrane can be described by classical transport equations describing diffusive and convective phenomena and 2)
transfer resistance of the gas stream boundary layer can be neglected under the operating conditions applied in this work.
4.2.- Performance of the pervaporation system After the preparation of the supported ionic liquid membrane stabilized by gelation, pervaporation tests were done under the same conditions of the membrane evaporation runs in order to quantify the membrane selectivity. Figure 8 shows the experimental extraction percentage for acetone, butanol and ethanol as a function of time for three different flow rate conditions. From these results, the extraction rates of each solute are completely different to the observed ones in membrane evaporation. In this case, the presence of the gelled supported ionic liquid membrane generates a preferential transport of butanol, reducing the overall transfer flux, but maintaining the order of magnitude of the fluxes observed in membrane evaporation (Figure 5). Although transport properties of IL gel gap are lower than the properties of the gas layer formed in the pores during the membrane evaporation process, the high solubility of these compounds, especially butanol and acetone, explains these flux values, which can be considered high if they are compared to typical fluxes through polymeric membranes. The partial flux obtained in this work for the supported gelled ionic liquid membranes is close to a mean value of 1.3x10-3 kg h-1 m-2 when butanol concentration was 500 ppm. Losses of IL were not observed during the pervaporation experiments. However, the membrane shows selectivity decreasing after 5 or 6 repeated pervaporation runs. Additional experiments were done with supported liquid ionic membranes without gelator and those membranes were not stable for the implementation of
pervaporation, since the liquid permeation of the ionic liquid was observed after the first minutes of operation. If we consider the ratio between the transmembrane flux and concentration gradient, the permeate flux obtained in this work is comparable or even higher with the values previously reported in the literature for pervaporation of ABE solutions with much higher feed butanol concentrations. Liu and coworkers  described the pervaporation of ABE mixtures using polymeric membranes based on PEBA 2533, which generate butanol fluxes ranging from 3.0x10-3 to 6.6x10-3 kg h-1 m-2 when the concentrations of the feed solution varied from 1030 to 1910 ppm, respectively. Zhou and collaborators  reported pervaporation trans-membrane butanol fluxes varying from 5.0x10-3 to 1.8x10-2 kg h-1 m-2 through hybrid silicalite-PDMS membranes when initial concentrations of butanol were between 10000 and 34000 ppm. These last values of concentrations are close or higher than the upper limit of butanol concentration in ABE fermentation broths [20-22]. On the other hand, Izák and coworkers  prepared pervaporation membranes based on PDMS containing the IL tetrapropylammonium tetracyanoborate, obtaining as much as 2.4x10-2 kg h-1 m-2 of butanol when concentration of the aqueous feed solution was 9000 ppm. The preferential transfer of butanol on acetone and ethanol can be explained by the solubility of these species in the IL membrane. Figure 9a shows the partition coefficients of acetone, butanol and ethanol obtained experimentally at 25ºC when the IL/aqueous volumetric ratio was 1:1. In order to obtain the partition coefficient, aqueous mixtures with known concentrations was mixed for each component with ionic liquid gels with 1:1 ratio using 1 mL of the solutions in the sealed vessels. After the equilibrium has been reached, the concentration of aqueous phase was analyzed in GC
while the concentration of the IL gel was calculated from a mass balance. After obtaining concentrations in each phase, the partition coefficient was calculated as a ratio of these concentrations. These values of partition coefficient show different equilibrium concentrations ratios when compared to membrane evaporation, which obeys to the Henry’s constant value of each compound. The presence of ionic liquid gel into the pores involves a similar dissolution of acetone and butanol in the membrane. The mean transmembrane flux of each compound for all pervaporation tests is reported in Figure 9b, and it is the evidence of this equilibrium condition between the aqueous feed solution and the IL gel. Thus, there is a direct relationship of the partition coefficient with the transmembrane flux obtained from the pervaporation experiments. However, the permeability of these compounds through the gelled ionic liquid membrane cannot be exclusively explained by the magnitude of individual partition coefficients and additional aspects related to the transport phenomena through the membrane and at the boundary layers formed in its proximities must be also considered. On the other hand, it was assumed that pores are filled with IL gel. However, this assumption could be a source of error when the transfer model is confronted to the experimental results. Anyway, with a significant number of empty pores in the pervaporation membrane its selectivity would be notoriously different and closer to the evaporation performance reported in this work.
4.3.- Selectivity in the pervaporation of ABE mixtures The selectivity of each compound can be quantified in terms of its comparative permeation flux. In this work, butanol/acetone and butanol/ethanol ratios were considered because the main interest in this type of process is the development of a novel technique for separation of butanol from fermentation broths. Transfer flux ratios
were calculated in order to show the preferential butanol permeation through the gelled IL membrane. Thus, Nbutanol/Nacetone ratio varied between 1.068 and 1.214 and Nbutanol/Nethanol ratio varied between 1.333 and 2.079. These flux ratios could be considered low in terms of selectivity under the operating conditions chosen for this study where initial concentrations are the same for all components (500 ppm). Anyway, these flux ratios are higher than the values obtained with membrane evaporation, where the non-selective membrane process shows mean ratios of 0.48 for butanol/acetone and 1.02 for butanol/ethanol. The relative flux of butanol could be increased if the relative concentration of butanol in the solution increases. If the magnitude of flux depends on the concentration gradient through the membrane, then a acetone/butanol/ethanol ratio of 3:6:1 considers approximately the same increasing of relative fluxes compared to the 1:1:1 ratio used in this study. In a real fermentation system, bio-butanol is generated by Clostridium bacteria, yielding 3 parts of acetone, 6 of butanol and 1 of ethanol. Thus, the selectivity could be significantly improved in a coupled fermentation reactor, since the driving force of the transfer through the gelled IL membrane would be highly favorable to butanol. Future tests will be done in the framework of this research in order to validate the improved selectivity in fermentation model solutions. Further research should be focused on the development and screening of more selective ionic liquids as well as the pilot plant tests in order to assess the membrane stability in function of time. Moreover, the membrane developed in this work could be used for butanol or acetone separation by pervaporation from other type of solutions, where the competitive extraction with other solutes is less significant. Nevertheless, a future research work is necessary in order to achieve a improved stabililty of the membranes and a detailed
quantification of the water transfer through the membrane. In this work, acetone, butanol and ethanol transfer was analyzed monitoring the concentration changes in the aqueous feed solution as a function of the time by means gas chromatography. In pervaporation and membrane evaporation tests this method showed low experimental variability. The same procedure was simultaneously applied for the permeate, which was condensated in a cold trap contained in a vessel with liquid nitrogen. The analysis of the condensate didn’t show the same reliability of the analysis results on the feed solution, especially for the estimation of acetone concentration. In those previous tests, the mass balance done on the volatile compounds showed losses of acetone close to 34% in the cold trap, probably dues to a unfavorable design of this apparatus. This procedure will be improved in future works to evaluate the selectivity of all compounds including water.
4.4.- Modeling of mass transfer in pervaporation and identification of controlling steps The mass transfer model described in sections 3.3 and 3.4 was developed for individual transport of each compound transferred through the gelled IL membrane. Physical and transport properties of the compounds in the fluid phases (liquid and gas) were collected from the literature. Density and viscosity of the aqueous feed phase containing 500 ppm of acetone, butanol and ethanol were supposed to be close to the values of pure water (993.63 kg m-3 and 8.11x10-4 Pa s) , meanwhile these same properties for the gas stream were estimated for pure nitrogen (1.11 kg m-3 and 1.86 Pa s)  at the operating conditions. The only unknown parameter in this modeling was the diffusion coefficient of each solute in the IL gel that filled the membrane pores. Thus, the model was used to correlate the diffusion coefficient of acetone, butanol and
ethanol in the gelled IL layer, identifying the value that generates the lowest meansquared errors with the experimental data. Figure 10 shows an example of these calculations. Diffusion coefficient values for each solute in the gelled IL layer were estimated from the experimental results using the simulation program developed in this study. In this way, simulations were done with different diffusion coefficient values until to obtain the minimum root mean square between simulated solute transfer fluxes and the experimental ones. The range of these values is reported in Table 4. From the results reported in Table 4 as well as in Figure 9, we can notice that even if the transport of species is given by a combination of two phenomena solubility and diffusion in the case of butanol, the global transport is mainly influenced by solubility and then by thermodynamics, instead of transport kinetics because butanol presents the lower diffusion coefficient of the three tested compounds. Meanwhile, ethanol transfer rate seems to be faster than the predicted by the partition coefficient ratio, since ethanol shows the highest diffusion coefficient in the IL gel layer. Indeed, the gelled IL membrane represents the main controlling step of mass transfer with a smaller effect of the liquid feed boundary layer. The solubility and transport properties of the solutes in the IL gel are the key parameters of the pervaporation process. This was verified by means of the estimation of the local resistance percentages described in section 3.1 by equations 10 and 11 for pervaporation and 18-20 for membrane evaporation. These local mass transfer resistances are reported in Figure 11. In our knowledge, the diffusion coefficients of acetone, butanol and ethanol in gelled ILs have not been reported yet. Furthermore, the diffusion coefficients of acetone, butanol and ethanol in [bmim][PF6] are not reported in the literature at room conditions. Voss and coworkers  proposed the formation of [hmim][Tf2N] gels with
12-hydroxysteraric acid (1.5% w/w) for light gas separation, finding slight decreasing of CO2 and N2 permeabilities with respect to pure IL. Moreover, Méndez-Morales and coworkers  report a diffusion coefficient value of ethanol in non-gelled [hmim][PF6] equal to 1.207x10-9 m2 s-1. If this value is used as reference, the diffusion coefficient estimated in this work for ethanol in gelled [bmim][PF6] is 55% lower; this difference can be explained by the effect of the gel formation on the transport properties of the IL. Besides, the diffusion coefficient values of butanol in IL membranes estimated in this work are approximately two times higher than the values reported by Vopicka and coworkers , who developed blended silicone–ionic liquid membranes based on poly(dimethylsiloxane)–benzyl-3-butylimidazolium
separation. Finally, Cascon and Choudhari  reported the pervaporation of aqueous butanol solutions with initial concentrations between 5000 and 25000 ppm at temperatures varying from 35 to 70ºC, using a supported liquid membrane prepared on CelgardTM flat sheet membranes with its pores filled of hydrophobic ammonium- and phosphonium-based ionic liquids, verifying a direct relationship between transmembrane fluxes and the absorption of butanol and water in the IL. These authors obtained diffusion coefficients of butanol in IL ranging between 2.0x10-11 and 8.0x10-11 m2 s-1. They reported high values of butanol flux (up to 0.8 kg h-1 m-2 at 70ºC), which can be explained by the use of a thin membrane support with a thickness of only 25 m. In the pervaporation system studied in this work, the membrane selectivity is given by a combination of solubility and diffusivity of the different compounds in the ionic liquid gel layer. The relatively faster flux of butanol can be explained by the higher solubility of this compound in the ionic liquid. Nevertheless, the fluid dynamic
conditions of the membrane module, with low Reynolds number values, involve a significant influence of the boundary layers at the proximities of the membrane on the overall mass transfer, which was observed in the experimental results.
5.- Conclusions In this work, pervaporation of aqueous ABE mixtures has been implemented by using supported gelled ionic liquid membranes based on [bmim][PF6] in order to separate butanol from the aqueous solution. Pervaporation assays were compared with membrane evaporation runs developed with the same experimental setup and membrane support without IL gel. The use of an IL gel layer formed with a low concentration of gelator generates membranes with a permeability comparable to a membrane evaporation system, but selective to the butanol transfer. The selectivity of the membrane is mainly given by the partition coefficient between the IL gel and the aqueous solution and the membrane itself seems to represent the main controlling transport step during the pervaporation process. A mass transfer model based on classical transport equations was proposed to describe the pervaporation process and the reference membrane evaporation system. This model allowed the simulation of the membrane evaporation system, verifying the chosen correlation for mass transfer coefficient in the aqueous ABE feed solution boundary layer. The same theoretical approach was applied for the pervaporation description. Thus, the model was used to correlate the diffusion coefficient of acetone, butanol and ethanol in the IL gel layer. The model is coherent with the experimental data and it is capable to correlate the mass transfer coefficients of each solute in the IL
gel layer, which are larger than the values reported for polymerized ILs or blended with polymers. These values are moderately lower than in similar non-gelled IL.
Acknowledgements The financial support of FONDECYT Project nº1100305, ECOS-CONICYT Program (Project C10E05) and Graduate Scholarship Program of CONICYT Chile is gratefully acknowledged. This study has been supported by Project ICM-P10-003-F, CILIS, granted by Fondo de Innovación para la Competitividad, del Ministerio de Economía, Fomento y Turismo, Chile.
kg m-2 h-1
Interfacial surface area for mass transfer
Total volume of feed solution
Local mass transfer coefficient
Surface area for mass transfer
Thickness of the hollow fiber support
A constant in Eq 13
Fiber packing fraction
Refers to aqueous phase
Refers to gaseous phase
Refers to pore filled with IL
Refers to logarithmic mean
Refers to interface
Refers to ionic liquid
Refers to the bulk of the feed solution
Refers to the bulk of the gaseous phase
Refers to the pore filled with gas
Refers to solute
Refers to membrane evaporation
Refers to sweeping gas pervaporation
References  C. Jin, M. Yao, H. Liu, C. F. Lee, J. Ji, Progress in the production and application of n-butanol as a biofuel, Renewable and Sustainable Energy Reviews 15 (2011) 4080– 4106.
 K. Kraemer, A. Harwardt, R. Bronneberg, W. Marquardt, Separation of butanol from acetone-butanol-ethanol fermentation by a hybrid extraction-distillation process, 20th European Symposium on Computer Aided Process Engineering – ESCAPE20.
 R. K. Sukumaran, L. D. Gottumukkala, K. Rajasree, D. Alex, A. Pandey, “Butanol Fuel from Biomass: Revisiting ABE Fermentation” in Biofuels: Alternative Feedstocks and Conversion Processes, 571-586.
 N. Qureshi , M.M. Meagher, J. Huang, R.W. Hutkins, Acetone butanol ethanol (ABE) recovery by pervaporation using silicalite–silicone composite membrane from fed-batch reactor of Clostridium acetobutylicum, Journal of Membrane Science 187 (2001) 93–102.
 J. Huang, M.M. Meagher,
Pervaporative recovery of n-butanol from aqueous
solutions and ABE fermentation broth using thin-film silicalite-filled silicone composite membranes, Journal of Membrane Science 192 (2001) 231–242.
 N. Qureshi, M.M. Meaghera, R.W. Hutkins, Recovery of butanol from model solutions and fermentation broth using a silicalite/silicone membrane, Journal of Membrane Science 158 (1999) 115-125.
 H. Zhou, Yi Su, Xiangrong Chen, Yinhua Wan, Separation of acetone, butanol and ethanol (ABE) from dilute aqueous solutions by silicalite-1/PDMS hybrid pervaporation membranes, Separation and Purification Technology 79 (2011), 375–384.
 J.D. Kawedia, V.G. Pangarkar, K. Niranjan, Pervaporative stripping of acetone, butanol and ethanol to improve ABE fermentation, Bioseparation 9 (2000) 145–154.
 E. Faver, T.Q. Nguyen, S. Bruneau, Extraction of 1-butanol from aqueous solutions by pervaporation, J. Chem. Technol. Biotechnol. 65 (1996) 221–228.
 A. Jonquieres, A.G. Fane, Filled and unfilled composite GFT PDMS membranes for the recovery of butanols from dilute aqueous solutions: influence of alcohol polarity, J. Membr. Sci. 125 (1997) 245–255.
 W.J. Groot, M.C.H. den Reyer, T.B. de la Faille, R.G. van der Lans, K.C. Luyben, Integration of pervaporation and continuous butanol fermentation with immobilized cells. I. Experimental results, Chem.Eng. J. Biochem. Eng. J. 46 (1991) B1–B10.
 A. Jonquieres, A.G. Fane, Filled and unfilled composite GFT PDMS membranes for the recovery of butanols from dilute aqueous solutions:influence of alcohol polarity, J. Membr. Sci. 125 (1997) 245–255.
 A. Friedl, N. Qureshi, I.S. Maddox, Continuous acetone–butanol–ethanol (ABE) fermentation using immobilized cells of Clostridium acetobutylicum in a packed bed
reactor and integration with product removal by pervaporation, Biotechnol. Bioeng. 38 (1991) 518–527.
 N. Qureshi., I.S. Maddox, A. Friedl, Application of continuous substrate feeding to the ABE fermentation. Relief of product inhibition using extraction, perstraction, stripping, and pervaporation, Biotechnol. Prog. 8 (1992) 382–390.
 E. A. Fouad, X. Feng, Use of pervaporation to separate butanol from dilute aqueous solutions: Effects of operating conditions and concentration polarization, Journal of Membrane Science 323 (2008) 428–435.
 F. Liu, L. Liu, X. Feng, Separation of acetone–butanol–ethanol (ABE) from dilute aqueous solutions by pervaporation, Separation and Purification Technology 42 (2005) 273–282.
 Y. K. Ong, N. Widjojo, T.S. Chung,
Fundamentals of semi-crystalline
poly(vinylidene fluoride) membrane formation and its prospects for biofuel (ethanol and acetone) separation via pervaporation, Journal of Membrane Science 378 (2011) 149– 162.
 G. Liu, W. Wei, H. Wu, X. Dong, M. Jiang, W. Jin, Pervaporation performance of PDMS/ceramic composite membrane in acetone butanol ethanol (ABE) fermentation– PV coupled process, Journal of Membrane Science 373 (2011) 121–129.
 L. Gongping, H. Dan, W. Wang, X. Fenjuan and J. Wanqin, Pervaporation Separation of Butanol-Water Mixtures Using Polydimethylsiloxane/Ceramic Composite Membrane, Chinese Journal of Chemical Engineering, 19 (2011) 40-44.
 P. Pfromm, V. Amanor-Boadu, R. Nelson, P. Vadlani, R. Madl, Bio-butanol vs. bio-ethanol: A technical and economic assessment for corn and switchgrass fermented by yeast or Clostridium acetobutylicum, Biomass and Bioenergy, 34 (2010) 515-524.
 V. García, J. Päkkilä, H. Ojamo, E. Muurinen, R. L. Keiski, Challenges in biobutanol production: How to improve the efficiency? Renewable and Sustainable Energy Reviews 15 (2011) 964–980.
 E.P. Knoshaug, M. Zhang, Butanol tolerance in a selection of microorganisms. Applied Biochemistry and Biotechnology 2009;153:13–20.
 R. Fortunato, C. A.M. Afonso, M.A.M. Reis, J. G. Crespo, Supported liquid membranes using ionic liquids: study of stability and transport mechanisms, Journal of Membrane Science 242 (2004) 197–209.
 F. J. Hernández-Fernández, A. P. de los Rios, M. Rubio, F. Tomás-Alonso D. Gómez, G. Villora, A novel application of supported liquid membranes based on ionic liquids to the selective simultaneous separation of the substrates and products of a transesterification reaction, Journal of Membrane Science 293 (2007) 73–80.
 S. H. Ha, N. L. Mai, Y.M. Koo, Butanol recovery from aqueous solution into ionic liquids by liquid–liquid extraction, Process Biochemistry 45 (2010) 1899–1903.
 L. D. Simoni, A. Chapeaux, J. F. Brennecke, M. A. Stadtherr, Extraction of biofuels and biofeedstocks from aqueous solutions using ionic liquids, Computers and Chemical Engineering 34 (2010) 1406–1412.
 A. P. de los Ríos, F. J. Hernández-Fernández, M. Rubio, D. Gómez, G. Víllora, Highly selective transport of transesterification reaction compounds through supported liquid membranes containing ionic liquids based on the tetrafluoroborate anion, Desalination 250 (2010) 101–104.
 F. J. Hernández-Fernández, A. P. de los Ríos, F. Tomás-Alonso, D. Gómez, G. Víllora, Improvement in the separation efficiency of transesterification reaction compounds by the use of supported ionic liquid membranes based on the dicyanamide anion, Desalination 244 (2009) 122–129.
 A. P. de los Ríos, F. J. Hernández-Fernández, F. Tomás-Alonso, M. Rubio, D. Gómez, G. Villora, On the importance of the nature of the ionic liquids in the selective simultaneous separation of the substrates and products of a transesterification reaction through supported ionic liquid membranes, Journal of Membrane Science 307 (2008) 233–238.
 P. Izák, W. Ruth, Z. Fei, P. J. Dysonc, U. Kragl, Selective removal of acetone and butan-1-ol from water with supported ionic liquid–polydimethylsiloxane membrane by pervaporation, Chemical Engineering Journal 139 (2008) 318–321.
 H. R. Cascon, S. K.Choudhari, G. M. Nisola, E. L. Vivas, D.J. Lee, W.J. Chung, Partitioning of butanol and other fermentation broth components in phosphonium and ammonium-based ionic liquids and their toxicity to solvent ogenic clostridia, Separation and Purification Technology 78 (2011) 164–174.
 B.A. Voss, J.E. Bara, D.L. Gin, D.R. Noble, Physically Gelled Ionic Liquids: Solid Membrane Materials with Liquid like CO2 Gas Tranport, Chem. Mater. 21 (2009) 3027-3029.
 K. Hanabusa, H. Fukui, M. Suzuki, H. Shirai, Specialist gelator for ionic liquids, Langmuir 21 (2005) 10383-10390.
 E. Pomier, N. Hengl, M.P. Belleville, D. Paolucci-Jeaniean, J. Sanchez, G. Rios, Study of a new metallic membrane evaporator, Desalination 199(2006) 185-187.
 N. Hengl, A. Mourgues, M.P. Bellevide, D. Paolucci-Jeanjean, J. Sanchez, Membrane contactor with hydrophobic metallic membranes: 2. Study of operating parameter in membrane operation, Journal of membrane science 355 (2010) 126-132.
 L. Tan, X. Dong, H. Wang, and Y. Yang, Gels of ionic liquid [C4mim][PF6] formed by self-assembly of gelators and their electrochemical properties, Electrochem. Commun. 11 (2009), 933-936.
 H.Estay, S. Bocquet, J. Romero, J. Sanchez, G.M. Rios, F. Valenzuela, Modeling and simulation of mass transfer in near-critical extraction using a hollow fiber membrane contactor, Chemical Engineering Science 62 (2007) 5794- 5808.
 A. Gabelman, S.T. Hwang, Hollow fiber membrane contactors, Journal of Membrane Science 159 (1999) 61-106.
 R. Prasad, K.K. Sirkar, Dispersion-free solvent extraction with microporous hollow-fiber modules, AIChE J. 34(2) (1988) 177-188.
 M. Mavroudi a, S.P. Kaldis b, G.P. Sakellaropoulos, A study of mass transfer resistance in membrane gas–liquid contacting processes, Journal of Membrane Science 272 (2006) 103–115
 S. Bocquet, J. Romero, J. Sanchez, G.M. Rios, Membrane contactors for the extraction process with subcritical carbon dioxide or propane: Simulation of the influence of operating parameters, Journal of Supercritical Fluids 41 (2007) 246-256.
 G. Bothun, B. Knutson, H. Strobel, S. Nokes, Mass transfer in hollow fiber membrane contactor extraction using compressed solvents, Journal of Membrane Science 227 (2003) 183-196.
 G. Wypych, Handbook of Solvents, ChemTec Publishing, Canada 2001.  R. H. Perry, D. W. Green, Perry's Chemical Engineer's Handbook, The McGrawHill Companies, Inc., 7th ed., 1999.  CHEMFATE. 1994. Syracuse Research Corporation's Environmental Fate Data Bases.
Syracuse Research Corporation, Syracuse, NY. U.S. ENVIRONMENTAL
PROTECTION AGENCY, Report 749-F-94-007a (Retrieved 8/15/94).
 T. Méndez-Morales, J. Carrete, M. García, O. Cabeza, L.J. Gallego, L.M. Varela, Dynamical Properties of Alcohol + 1-Hexyl-3-methylimidazolium Ionic Liquid Mixtures: A Computer Simulation Study, The Journal of Physical Chemistry B, 115(2011) 15313-15322.
 O. Vopika, V. Hynek, K. Friess, P. Izák, Blended silicone-ionic liquid membranes: transport of butan-1-ol vapor, European Polymer Journal 46 (2010) 123-128.
 H. R. Cascon, S. K. Choudhari, 1-Butanol pervaporation performance and intrinsic stability of phosphonium and ammonium ionic liquid-based supported liquid membranes,
LIST OF FIGURES
Figure 1. Cross section of hollow fiber support containing gelled ionic liquid immobilized into the pores of the membrane.
Figure 2. Experimental setup used in this work for pervaporation and membrane evaporation tests.
Figure 3.Outline of the mass transfer principle in the (a) pervaporation process (b) membrane evaporation process studied in this work at the proximities of the membrane.
Figure 4. Flowchart of the algorithm for calculation of mass transfer flux of solutes in pervaporation and membrane evaporation processes using a resistances-in-series model
Figure 5.Experimental extraction percentage of membrane evaporation of acetone, butanol and ethanol as a function of the time for different flow rates of liquid feed solution and sweeping gas stream: a) 1.17*10-5 L s-1 of feed solution and 5.0*10-3 L s-1 of N2; (b) 4.33*10-5 L s-1 of feed solution and 5.0*10-3 L s-1 of N2; (c) 4.33*10-5 L s-1 of solution and 2.17*10-2 L s-1 of N2.
Figure 6.a) Henry’s law constant values for each solute  and b) the mean cumulative transmembrane solute flux (kg m-2 h-1) of the three different experimental runs of membrane evaporation reported in Figure 5.
Figure 7. Experimental and simulated concentration change rate for membrane evaporation of acetone, butanol and ethanol with a flow rate of 1.17*10-5 L s-1 and 5.0*10-3 L s-1 of feed solution and sweeping gas stream, respectively. Initial concentration (C0) of each solute was 500 ppm.
Figure 8. Experimental extraction percentage of pervaporation of acetone, butanol and ethanol as a function of the time for different flow rates of liquid feed solution and sweeping gas stream: a) 1.17*10-5 L s-1 of feed solution and 5.0*10-3 L s-1 of N2; (b) 4.33*10-5 L s-1 of feed solution and 5.0*10-3 L s-1 of N2; (c) 4.33*10-5 L s-1 of solution and 2.17*10-2 L s-1 of N2.
Figure 9.a) Partition coefficients of acetone, butanol and ethanol between the IL gel and the aqueous feed solution at 25ºC with a phase volumetric ratio of 1:1 when the initial solute concentration in the aqueous phase was 500 ppm; b) the mean cumulative transmembrane solute flux (kg m-2 h-1) of the three different experimental runs of pervaporation reported in Figure 8.
Figure 10.Experimental and correlated concentration change rate for pervaporation of acetone, butanol and ethanol with a flow rate of 1.17*10-5 L s-1 and 5.0*10-3 L s-1 of feed solution and sweeping gas stream, respectively. Initial concentration (C0) of each solute was 500 ppm.
Figure 11. Local mass transfer resistances calculated in terms of the percentage of overall resistance for the sweep gas pervaporation and membrane evaporation processes.
LIST OF TABLES
Table 1. Structural parameters of the fiber and module used in pervaporation and membrane evaporation experiments. PARAMETER
Table 2. Operating conditions forpervaporation and membrane evaporation experiments. Variable
Feed solution flow rate
1.2 x10-3-3.0 x 10-3
Concentration of solute
Volume of feed solution
2.3 x 10-2
Sweeping gas flow rate
Table 3. Physical properties of the ABE components [43, 44] Compound
(g mol )
25 C (g L )
25 0C (mmHg)
Table 4. Diffusion coefficient values of acetone, butanol and ethanol in IL gel layer. Values estimated by correlation of experimental data with the mass transfer model implemented for pervaporation. Compound Ds-IL gel [m2 s-1], range Acetone
4.6x10-10 - 4.9x10-10
3.9x10-10 - 4.2x10-10
5.2x10-10 – 5.6x10-10
݁݃ܽݐ݊݁ܿݎ݁݊݅ݐܿܽݎݐݔܧሺΨሻ ൌ ܰௌா ൌ
ൌ ݇ ܵை ሺܥௌǡଶ െ ܥௌǡ ሻ
ଵ ೌ ௗವ
ಽ షಽௗಽಾ ೌ
భ ೖೌ ವ భ ಼ ೡೌ ವ
భ ಼ ಽ ೖషಽ ಽಾ ೌ భ ಼ ೡೌ ವ
݄ܵ ൌ ͳǤʹ ቀܴ݁ ܵܿ ௗೀವ
݄ܵ ൌ ߚ ቂ ܪ ൌ ೌ
ሺͳ െ ߮ሻቃ ൫ܴ݁Ǥ ܵܿǤଷ ൯
( ͲͲͳ כ1)
ܭಽ ൌ ሺሻ
ൌ ݇ିூ ܵெ ሺܥௌǡଵ െ ܥௌǡଶ ሻ
ൌ ݇ ܵூ ሺܥௌǡ െ ܥௌǡଵ ሻ
ܭಽ ൌ ሺூሻ
ሺೄǡ ሺ௧ୀሻିೄǡ ሺ௧ሻሻ
ܵெ ቀܥௌǡଵ െ ܥௌǡைோா ቁ
ൌ ݇ ܵை ቀܥௌǡைோா െ ܥௌǡ ቁ
ଵ ௗ ಾಶ ವ
ଵ ೌ ௗವ
భ ೖೌ ವ భ ಼ ಾಶ ವ
ഄವೄǡ ൰ௗಽಾ ு൬ ഓಽ ೌ
ଵ ு ௗೀವ
భ ഄವೄǡ ಹቆ ഓಽ ቇಽಾ ೌ భ ಼ ಾಶ ವ
భ ಹ ೖ ೀವ ೌ భ ಼ ಾಶ ವ
1. Separation of ABE mixtures by pervaporation with gelled IL membranes 2. Supported IL membranes were stabilized with a low-molecular-weight gelator 3. Diffusion coefficient in the membrane was estimated using a transfer model 4. Pervaporation tests were compared to membrane evaporation process 5. Transfer rates are governed by the solubility of solutes in the IL membrane